Upcoming SlideShare
×

Thanks for flagging this SlideShare!

Oops! An error has occurred.

×
Saving this for later? Get the SlideShare app to save on your phone or tablet. Read anywhere, anytime – even offline.
Standard text messaging rates apply

# Introduction Quantitative X-Ray Diffraction Methods

2,311

Published on

0 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• Be the first to comment

• Be the first to like this

Views
Total Views
2,311
On Slideshare
0
From Embeds
0
Number of Embeds
0
Actions
Shares
0
50
0
Likes
0
Embeds 0
No embeds

No notes for slide

### Transcript

• 1. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010)IntroductionQualitative analysis usually involves the identification of a phase or phases in a specimen bycomparison with “standard” patterns (i.e., data collected or calculated by someone else), andrelative estimation of proportions of different phases in multiphase specimens by comparingpeak intensities attributed to the identified phases.Quantitative analysis of diffraction data usually refers to the determination of amounts ofdifferent phases in multi-phase samples. Quantitative analysis may also be thought of interms of the determination of particular characteristics of single phases including precisedetermination of crystal structure or crystallite size and shape. In quantitative analysis, anattempt is made to determine structural characteristics and phase proportions withquantifiable numerical precision from the experimental data itself. Though “standard”patterns and structural data are used as a starting point, the most successful quantitativeanalysis usually involves modeling the diffraction pattern such that the calculated pattern(s)duplicates the experimental one.All quantitative analysis requires precise and accurate determination of the diffraction patternfor a sample both in terms of peak positions and intensities. While some kinds of analysis(i.e., particle shape and clay structure) rely on the existence of preferred orientation, mostrequire a uniformly sized, randomly oriented fine (ideally 1-2 m) powder specimen toproduce intensities which accurately reflect the structure and composition of the phase(s)analyzed.As will become evident, the successful application of quantitative methods requires carefulsample preparation, good quality data and a very thorough understanding of the material youare working with and the possible sources of error in your experiments. Since diffractiondata are generally very dependent on the systematics of your diffractometer and its datacollection system, application of quantitative methods that involve ratios of peak intensitiesrequires careful calibration with well-known standards before a quantitative analysis isattempted.The most effective quantitative methods, particularly those involving pattern modeling, arecomputationally intensive can only be applied with powerful analytical software.Commercial versions of this type of software are very expensive. Fortunately there areseveral inexpensive (or free) versions of software to do pattern refinements and quantitativeanalysis. Though they are not as “user friendly” as the commercial versions, once thelearning curve is climbed, they can be very effective analytical tools.This chapter will focus on approaches to quantitative determination of the amounts ofparticular phases in multiphase samples. At best this chapter is a skimpy introduction to avery large field. The basic organization is modified from Chapter 13 of Jenkins and Snyder(1996). The last section, essential for anyone wanting to apply these methods to their ownwork, is a partial list of reference material related to quantitative methods.The Intensity EquationThe diffraction pattern includes information about peak positions and intensity. The peakpositions are indicative of the crystal structure and symmetry of the contributing phase. The (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 1 of 14
• 2. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010)peak intensities reflect the total scattering from the each plane in the phase’s crystal structure,and are directly dependent on the distribution of particular atoms in the structure. Thusintensities are ultimately related to both the structure and composition of the phase.The diffraction intensity equation has been described previously, and is summarized below. 2 I0 3 e2 M ( hkl ) 2 1 cos 2 (2 ) cos 2 (2 m ) v I ( hkl ) F( hkl ) 64 r me c 2 V2 sin 2 cos hkl swhere: I (hkl ) = Intensity of reflection of hkl in phase . I 0 = incident beam intensity r = distance from specimen to detector = X-ray wavelength (e 2 / mc 2 ) 2 = square of classical electron radius s = linear absorption coefficient of the specimen v = volume fraction of phase Mhkl = multiplicity of reflection hkl of phase 0 = Lorentz-polarization (and monochromator) correction (next to last term to right) v = volume of the unit cell of phase 2 m = diffraction angle of the monochromator F(hkl) = structure factor for reflection hkl of phase (i.e., the vector sum of scattering intensities of all atoms contributing to that reflection).Recognizing that many of these terms are consistent for a particular experimental setup wecan define an experimental constant, Ke. For a given phase we define another constant,K(hkl) , that is effectively equal to the structure factor term for phase . Substituting theweight fraction (X ) for the volume fraction, the density of the phase ( ) for the volume, andthe mass absorption coefficient of the specimen ( / )s for the linear absorption coefficientyields the following equation: K e K ( hkl ) X I ( hkl ) ( / )sThis equation describes in simpler terms the intensity for peak hkl in phase .The fundamental problem (aside from the non-trivial problem of getting accurate intensitymeasurements from a homogeneous randomly oriented powder) lies in the mass absorptioncoefficient for the sample, ( / )s. If this quantity is known, the calculations are simple. Theproblem is that in most experiment ( / )s is a function of the amounts of the constituentphases and that is the object of our experiment. Basically, all of the peak intensity-relatedmethods for doing quantitative analysis discussed subsequently involve circumventing thisproblem to make this equation solvable. (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 2 of 14
• 3. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010)Sample Preparation IssuesWith the possible exception of whole-pattern (Rietveld and similar) methods of quantitativeanalysis (in which specimen characteristics become another parameter to be modeled),successful quantitative analysis requires a specimen that presents a very large number ofrandomly oriented, uniformly sized crystallites to the X-ray beam. Preparation of specimensthat start out as large solid objects (i.e., rocks, ores, concrete, ceramics, etc.) for quantitativeanalysis will usually involve a multi-phase process involving a variety of equipment. Mostof the equipment currently available in the Department of Earth and Planetary Sciences arelisted in the chapter on “Errors and Sample Preparation” (p. 12-13).The statistics of particle size and consequent statistical errors in intensities determined by adiffractometer have been discussed previously in the chapter on “Errors and SamplePreparation” (p. 8-10). The point of this discussion is that to achieve peak intensity errors ofless than 1% for a single phase (100% of specimen) requires particles between 0.5 and 1.0 m in size. This particle size range, in practice is extremely difficult to obtain. The bestmethods generally result in a 1-5 m size range, and the statistics are further degraded by thefact that every phase in a multi-phase sample will be less than 100% of the whole. All of thismeans that a statistical error of 5% for major phases in an intensity-related quantitativeanalysis should be considered reasonable. Be suspicious of analyses that report lower errors.All of the errors related to sample preparation discussed in the previous chapter may be afactor in quantitative analysis. Clearly the most successful quantitative analyses will be withmaterials in which particle size is uniform, small and well known; engineered materialsfrequently fall into this category.Particular caution must be exercised in situations where crystallite sizes vary widely within aparticular sample; many rocks and most soils fall into this category. The author worked formany years with extrusive volcanic rocks from southern Nevada. These pyroclastic rocksincluded non-welded vitric and zeolitized fall and flow deposits and very densely weldeddevitrified ash-flow tuffs. A goal of the analyses was to produce repeatable quantitativedeterminations of the amounts of different phases in the specimens. Although techniqueswere developed using an internal standard that could produce repeatable results ( 5%) inknown binary mixtures, the method could not be successfully applied to the actual rocks andresults varied by up to 30% from independent determinations with petrographic microscope,electron microprobe and chemical techniques. The most likely root of this failure was theinability to produce homogeneous crystallite sizes in source materials containing a widerange of constituents (from <<1 m devitrification products to 50+ m pore fillingcrystallization products to 1-2 mm phenocrysts of quartz and feldspar).An excellent and concise reference summarizing most of what you need to know aboutsample preparation for all purposes in XRD (including quantitative analysis) is the article byBish and Reynolds in Bish and Post (1989).Measurement of Line IntensitiesAll of the methods of quantitative analysis (even whole-pattern methods) require accurateintensity measurements. The table below (from Jenkins and Snyder, p. 356) summarizes thevarious factors which control absolute and relative intensities in a powder pattern. (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 3 of 14
• 4. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010)Structure Sensitive Factors: These factors are mostly included in the K(hkl) term in theintensity equation. Most of these factors are intrinsic properties of the phase producing thereflection, but their intensity can be modified both temperature and the wavelength of theincident radiation.Factor Parameter1. Structure-sensitive Atomic scattering factor Structure factor Polarization Multiplicity Temperature2. Instrument-sensitive Source Intensity (a) Absolute intensities Diffractometer efficiency Voltage drift Takeoff angle of tube Receiving slit width Axial divergence allowed (b) Relative intensities Divergence slit aperture Detector dead time3. Sample-sensitive Microabsorption Crystallite size Degree of crystallinity Residual stress Degree of particle overlap Particle orientation4. Measurement-sensitive Method of peak area measurement Degree of peak overlap Method of background subtraction K 2 stripping or not Degree of data smoothing employedInstrument-sensitive Parameters: Variation in power supplied to the X-ray tube can causenotable variation in incident beam intensity over time. Fortunately most modern digitalpower supplies (including our Spellman DF3 unit) include very sophisticated circuitry tovirtually eliminate voltage drift. All X-ray tubes will decrease in intensity as they age,however, and it is important to monitor this over time.Detector dead time can cause very intense peaks to be measured with lower intensity; theproper dead time correction should be applied to correct your data for this.Sample-sensitive Parameters: These are by far the most important class of factors affectingquantitative work. All of these factors have the capability of severely compromising theusefulness of your diffraction data. Bottom line: keep your crystallite size at 1 m for all (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 4 of 14
• 5. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010)phases and eliminate preferred orientation in your specimen and you’ve got a chance ofgetting usable data.Measurement-sensitive Parameters: The selection of the 2 points at which backgroundwill be measured is critical to determination of accurate integrated peak intensities. Thechoice of where the peak starts and ends relative to background will have a significant effect on integrated intensity as illustrated in the figures (from Jenkins and Snyder, 1996) below. Figure 13.3 shows an experimental trace of the (111) peak of Si using Cr radiation. Note that the peak has a notable “tail” and the start of the peak could be picked at some point between 41.5 and 42.2 2 . The RIR is the ratio between the integrated intensities of the peak of interest and that of a known standard (Corundum in this case). Figure 13.4 shows how the RIR varies as a function of where the background is picked (holding the Al2O3 line constant). Clearly, where thebackground is picked will have a significant effect on peak ratios, and thus the amount of theunknown determined.It must be noted that peak areas for well-defined peaks will be proportional to peak heights,but that this relationship breaks down in peaks which show significant broadening. Asdiscussed previously in the material on diffraction intensities (Diffraction Basics Part 2 –Week 6), peak broadening, either by strain or particle size, results in integrated peakintensities (generally larger) which are not representative of the amounts present, thus somesort of correction for this broadening is desirable for quantitative analysis. This effect isshown in the left-most two peaks in (Fig.13.5a and 13.5b below). (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 5 of 14
• 6. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010)Another significant problem in the use of integrated intensities is in overlapping peaks ofinterest and the difficulty of calculating integrated intensities. This requires one of twoapproaches: selection of peaks which do not overlap or decomposition of overlapping peaksinto their components prior to calculating integrated intensities. The peak overlap situation isshown in Figure 13.5c below. Sophisticated digital tools for processing diffraction datamake peak deconstruction or “deconvolution” possible.Useful tools in Jade to assist in processing Intensity MeasurementsThe routine peak identification routine in Jade is useful for quick location of prominent peaksin a pattern, however the peak intensity determinations done by this routine are generallyinadequate to intensity calculation required for quantitative analysis. Jade includes a numberof processing tools which can assist in processing XRD patterns to obtain good reducedintensity data for software has several tools that are very effective in processing diffractiondata to obtain background-corrected peak intensities for overlapping peaks. It should benoted that Jade does not alter the original data file when refining your data, but createsseparate overlays that modify the data as used and displayed. Some of the useful intensity-related tools are: Background and K 2 Removal (Flexible tool for removing background) Profile Fitting and Peak Decomposition (Interactive tool for differentiating and separating overlapping peaks) Crystallite Size and Strain Analysis from Peak Broadening (Tool used with standard materials – NIST 640b Si or LaB6 – to establish instrumental broadening parameters and evaluate peak broadening from strain and crystallite size)Quantitative Methods based on Intensity RatiosNumerous methods have been developed to use peak intensities for quantitative analysis ofdiffraction data. Many of them are specialized in nature (i.e., require binary mixtures or (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 6 of 14
• 7. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010)involve polymorphs having the same mass absorption coefficients). Jenkins and Snyder(1996) introduce most of these methods, some of which are included here. By far themethods in most general use involve addition of a known amount of an internal standard andcalculating ratios of the areas of the standard peaks to those of the phases being determined.The Absorption-Diffraction MethodThe absorption-diffraction method involves writing the diffraction equation twice – once forthe phase in the sample and once for the pure phase, and then dividing the equations to yield: I ( hkl ) ( / ) 0 X I ( hkl ) ( / )swhere I0 is the intensity of the peak in the pure phase. For most materials, the massabsorption coefficient of the mixture remains the undeterminable unknown. In thespecialized case where ( / )s is the same as the phase being determined (as in isochemicalpolymorphs) this equation reduces to the simple case: I ( hkl ) X I (0hkl )A special case of this method for binary mixtures in where ( / ) for each pure phase isknown allows calculation of the amounts of both phases without requiring ( / )s using thefollowing equation: ( I ( hkl ) / I (0hkl ) )( / ) X ( / ) ( I ( hkl ) / I (0hkl ) )[( / ) ( / ) ]This equation is known as the Klug equation after H.P. Klug who first formulated it. As acheck on accuracy, it is possible to make the calculation for each phase independently andcompare results.The general case of the absorption-diffraction method requires that the mass absorptioncoefficient of the sample be known. This quantity can be experimentally determined by avariety of methods and used in the calculations. While theoretically possible, in generalerrors involved in this measurement are too large to be practically useful for quantitativeXRD.Since mass absorption is largely a function of atomic scattering, ( / )s may be estimatedfrom atomic scattering factors if the bulk chemistry of a sample is known. Tables ofelemental mass attenuation coefficients are published in the International Tables for X-RayCrystallography (and reproduced in most XRD texts) can be used to estimate the bulkcoefficient with reasonable accuracy. This then allows the generalized absorption-diffractionequation to be used directly.Method of Standard AdditionsThis method requires a variety of diffraction patterns run on prepared samples in whichvaried amounts of a well-known standard, , are added to the unknown mixture containingphase , the each mixture is analyzed . This method was developed and still widely used for (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 7 of 14
• 8. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010)elemental analysis by X-ray Fluorescence. Because of tedious sample preparation and dataerrors encountered at low concentrations of both phases, this is seldom applied in X-raydiffraction.Internal Standard MethodThe internal standard method, or modifications of it, is most widely applied technique forquantitative XRD. This method gets around the ( / )s problem by dividing two intensityequations to yield: I ( hkl ) X k I ( hkl ) Xwhere is the phase to be determined, is the standard phase and k is the calibrationconstant derived from a plot of I(hkl) / I(hkl) vs. X / X . Direct application of this methodrequires careful preparation of standards to determine the calibration curves, but can producequantitative determinations of identified phases that are substantially independent of otherphases in the specimen.Care must be taken when choosing standards to select materials with reasonably simplepatterns and well-defined peaks that do not overlap peaks in phases of interest. It is also veryimportant that the crystallite size of the specimen and standard be the same, ideally about 1 m.Reference Intensity Ratio MethodsI/Icorundum: It is clear from the internal standard equation above that a plot of I ( hkl ) X vs. X I ( hkl )will be a straight line with slope k. Those k values using corundum as the phase in a 50:50mixture with the phase are now published for many phases in the ICDD PowderDiffraction file, where I(hkl) is defined as the 100% line for both phases. In the PDF “card”this is defined as I/Ic, the reference intensity ratio for a 50:50 mixture of phase andcorundum. Ideally this provides a quick resource for quantitative determinations. Inactuality, use of published I/Ic values for quantitative analysis usually falls short because ofproblems with preferred orientation, inhomogeneity of mixing and variable crystallinity.Using multiple lines from corundum (with RIRs calculated from relative intensities) cancircumvent some of these problems by pointing out inconsistencies related to preferredorientation and other specimen irregularities. Use of experimentally determined RIR valuesrather than “published” values can greatly improve the accuracy of the results. For lab userswanting to use corundum as an internal standard, we have a significant quantity of 1 mCorundum from the Linde Division of Union Carbide available for use.Generalized RIR Method: In actual practice, reference intensity ratios (RIRs) can bedefined for any reference phase using any diffraction line. I/Ic is actually just a specializedRIR where hkl (and hkl´) are defined as the 100% line for the phase of interest andcorundum. The most general definition of the RIR for phase to reference phase is: (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 8 of 14
• 9. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010) I ( hkl ) I (rel ) hkl X RIR , rel I ( hkl ) I ( hkl ) XThe Irel term ratios the relative intensities of the peaks used; if the 100% peaks of both phasesare used, the value of this term is 1. RIRs may be experimentally determined for any phaseusing any material as a standard. Al2O3 (corundum) and SiO2 (quartz) are commonly used asinternal standards. ZnO is a popular internal standard with very good peaks. Multiple RIRsmay be calculated for different peaks in the same phases to provide a method for redundantdeterminations as a check on accuracy.RIRs may be determined for a variety of materials using different standards. RIRs carefullydetermined in the same laboratory under the same conditions as diffraction experiments canbe used to produce good, repeatable analyses. In addition, having good RIRs “in the can”permits the choice of the best standard (with minimal peak overlaps) for your specimen.Quantitative Analysis with RIRs: Rearranging the equation above yields the following: I ( hkl ) I (rel ) hkl X X I ( hkl ) I (rel ) hkl RIR ,The RIR value may be obtained through careful calibration, determination of the slope of theinternal standard plot or from other RIR values by: RIR , RIR , RIR ,Note that this equation allows any determined RIR (including I / Ic) to be used as long as ithas been determined for both phases. Best results will be obtained if as many as possible ofthe variables (the RIRs and the Irel values) are experimentally determined. The morepublished values that are used, the more the results must be considered semi-quantitativebecause of likelihood of significant errors.Note that because each phase determination is independent of the whole, this method willwork for complex mixtures including unidentified or amorphous phases.Normalized RIR Method: Chung (1974) recognized that if all phases in a mixture areknown and if RIRs are known for all of those phases, then the sum of all of the fractions ofall the phases must equal 1. This allows the writing of a system of n equations to solve forthe n weight fractions using the following summation equation: I ( hkl ) 1 X rel # phases RIR I ( hkl ) j 1 ( I ( hkl ) j / RIR j I (rel ) j ) hklChung referred to this method as the matrix flushing or adiabatic principle, but it is nowalmost universally referred to as the normalized RIR method, and allows “quantitative”calculations without the presence of an internal standard. It should be noted that thepresence of any unidentified or amorphous phases invalidates the use of this method. Itshould be further noted that in virtually all rocks, there will be phases in the sample thatare undetectable and thus the method will never rigorously work. (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 9 of 14
• 10. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010)Constrained XRD Phase Analysis: If independent chemical or other information about theconstituents in a sample is available, this information may be quantified and added toquantitative experimental data to constrain the results. The article by Snyder and Bish (inBish and Post, 1989) discusses the general rationale for how to approach analysis with thistype of complimentary data.Full-Pattern Analysis – the Rietveld MethodAdvances in computer technology have placed the computing power of the large mainframesystems of 30 years ago on virtually everyone’s desktop. The availability of this computingpower (and the diligence of a lot of dedicated computer programmers) has enableddiffractionists to work with the whole XRD pattern instead of just the relative intensities of afew identified peaks. Whole-pattern analyses are predicated on the fact that the diffractionpattern is the sum total of all of the effects, both instrumental and specimen-related, that wehave discussed earlier in our sections on “Diffraction Basics.” The basic approach is get thebest data you can (with or without an internal standard), identify all the phases present andinput basic structural data for all phases, then let the computer model your data until the bestfit to the experimental pattern is obtained.The Rietveld method was originally conceived as a method of refining crystal structuresusing neutron powder diffraction data. The method requires knowledge of the approximatecrystal structure of all phases of interest in the pattern. The quantity minimized in Rietveldrefinements is the conventional least squares residual: 2 R w j I j (o) I j (c) jwhere Ij(o) and Ij(c) are the intensity observed and calculated, respectively, at the jth step in thedata, and wj is the weight. Detailed discussion of the Rietveld method is way beyond thescope of this brief introduction, but it is important to understand that this method, becauseof the whole-pattern fitting approach, is capable of much greater accuracy and precisionin quantitative analysis than any peak-intensity based method.In Rietveld analysis, if an internal standard is used it is utilized to calibrate the scale factorsused by the program to match the model and experimental data, not to compare with thephases being analyzed. A “normalized” fit can be performed without an internal standard,but as with Chung’s normalized RIR method, the refinement will not usually succeed ifsomething is missing.Since the refinement “fits” itself to the data by modifying structure and instrumentparameters iteratively, the Rietveld method holds several advantages over other peakintensity-based methods: Differences between the experimental standard and the phase in the unknown are minimized. Compositionally variable phases are varied and fit by the software. Pure-phase standards are not required for the analysis. Overlapped lines and patterns may be used successfully. Lattice parameters for each phase are automatically produced, allowing for the evaluation of solid solution effects in the phase. (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 10 of 14
• 11. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010) The use of the whole pattern rather than a few select lines produces accuracy and precision much better than traditional methods. Preferred orientation effects are averaged over all of the crystallographic directions, and may be modeled during the refinement.The reader is referred to the referenced literature at the end of this chapter to dig deeper intothe Rietveld method. There is also information in this section about GSAS and RockJock,two free software systems capable of doing whole-pattern refinements for quantitativeanalysis.The Variables of a Rietveld Refinement: I will conclude here with a very qualitativeoutline of the factors which are entered by the analyst and varied by the analytical software toattempt a least squares fit to the experimental pattern.Refer to any of the references at the end of this chapter for a mathematical treatment; Snyderand Bish (1989) are particularly concise. Dr. Rietveld’s 1969 paper (available online athttp://crystal.tau.ac.il/xtal/paper2/paper2.html) provides as good an introduction as you willfind to the procedure. Peak shape function describes the shape of the diffraction peaks. It starts from a pure Gaussian shape and allows variations due to Lorentz effects, absorption, detector geometry, step size, etc. Peak width function starts with optimal FWHM values and Preferred orientation function defines an intensity correction factor based on deviation from randomness The structure factor is calculated from the crystal structure data and includes site occupancy information, cell dimensions, interatomic distances, temperature and magnetic factors. Crystal structure data is usually obtained from the ICDD database or other source (see references at end of chapter). As with all parameters in a Rietveld refinement, this data is a starting point and may be varied to account for solid solution, variations in site occupancy, etc. The scale factor relates the intensity of the experimental data with that of the model data.The least squares parameters are those varied in the model to achieve the best fit to theexperimental data and include two groups: The profile parameters include: half-width parameters, counter zero point, cell parameters, asymmetry parameter and preferred orientation parameter. The structure parameters include: overall scale factor, overall isotropic temperature parameter, coordinates of all atomic units, atomic isotropic temperature parameter, occupation number and magnetic vectors of all atomic units, and symmetry operators.All parameters require initial values be entered. This requires some thought on the part ofthe analyst to choose starting values that are reasonable for the phases analyzed. Therefinement program then varies the parameters in an attempt to minimize the differencebetween the experimental and calculated patterns using standard least-squares methods. (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 11 of 14
• 12. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010)Should the values chosen be very far off, it is not unusual for the refinement to blow up andnot converge on a solution. Fortunately, thanks to the speed of today’s computers, this willusually result in the loss of several minutes of work rather than a few days or weeks, andparameters may be revised and rerun relatively quickly.Detection Limit IssuesAn important consideration in any analysis of multiphase samples is the question of the lowerlimit of detection: What is the smallest amount of a given phase that can be identified in agiven X-ray tracing? The equation below defines the net counting error (n): 100[( N p N b )1 / 2 ] ( n) Np Nbwhere Np is the integrated intensity of the peak and background, and Nb is the backgroundintensity. As is obvious from this equation, as Np - Nb approaches zero, counting errorbecomes infinite. The equation describing the error in N is: (N ) N ( Rt )With R the count rate (c/s) and t the count time. Thus detection limits will clearly depend onthe square root of the count time.In the example shown above, the average background is 50 c/s and the 2 (95% probability)errors are shown for t = 10, 5, 1, and 0.5 s. Thus, with an integration time of 5 s, any countdatum greater than 55.3 c/s (6.3 c/s above background) would be statistically significant.The significance of this detection limit is dependent on the counts produced by a phase ofinterest at a particular concentration. In this example, if determining -SiO2 in an airbornedust sample, and a 5% standard gave 1,550 counts at the position of the (101) line with a 50 (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 12 of 14
• 13. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010)c/s background, then 1% -SiO2 would produce 300 c/s (1500 – 50 / 5). Thus the lowerdetection limit (2 ) will be 0.015% for 10s, 0.021% for 5s, 0.047% for 1s and 0.067% for0.5s.This exercise shows that given a known background level and counts produce by a knownconcentration of a phase, it is relatively easy to calculate the lower limit of detection for thatphase.Selected Resources for Quantitative AnalysisBish, D.L, and Howard, S.A., 1988, Quantitative phase analysis using the Rietveld method. J. Appl. Crystallography, v. 21, p. 86-91.Bish, D.L., and Chipera, S. J, 1988, Problems and solutions in quantitative analysis of complex mixtures by X-ray powder diffraction, Advances in X-ray Analysis v. 31, (Barrett, C., et al., eds.), Plenum Pub. Co., p. 295-308.Bish, D.L., and Chipera, S.J., 1995, Accuracy in quantitative x-ray powder diffraction analyses, Advances in X-ray Analysis v. 38, (Predecki, P., et al., eds.), Plenum Pub. Co., p. 47-57Chipera, S.J, and Bish, D.L, 1995, Multireflection RIR and intensity normalizations for quantitative analyses: Applications to feldspars and zeolites. Powder Diffraction, v. 10, p. 47-55.Chung, F.H., 1974, Quantitative interpretation of X-ray diffraction patterns. I. Matrix- flushing method of quantitative multicomponent analysis. Jour. of Applied Crystallography, v. 7, p. 519-525.Downs, R.T., and Hall-Wallace, M., 2003, The American Mineralogist crystal structure database. American Mineralogist, v. 88, p. 247-250. Comment: If you want structural data for minerals for your Rietveld refinements, this free online source has structural data for every experimentally determined structure published in the Journal (2,627 of them). This article explains the structure of the database, how to access it, and software available to help you make use of it. It is all online at: http://www.minsocam.org/MSA/Crystal_Database.html.Snyder, R.L. and Bish, D.L., 1989, Quantitative Analysis, in Bish, D.L. and Post, J.E., eds., Modern Powder Diffraction, Mineralogical Society of America Reviews in Mineralogy, V. 20, p. 101-144. Comment: A very concise and comprehensive introduction in an excellent volume, includes discussion of Internal Standard RIR methods and Rietveld methods. The chapter by Bish and Reynolds on Sample Preparation is also excellent.Young, R.A., 1993, The Rietveld Method, Intl. Union of Crystallographers Monograph on Crystallography V. 5, Oxford University Press, 298 p. Comment: Comprehensive Monograph on all aspects of Rietveld refinements. Very valuable for anyone planning apply seriously apply the technique.Chapter 13 in Jenkins and Snyder (1996) is also recommended as good introductory reading on quantitative methods. (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 13 of 14
• 14. Introduction Quantitative X-Ray Diffraction Methods (prepared by James R. Connolly, for EPS400-001, Introduction to X-Ray Powder Diffraction, Spring 2010)Free Software for Quantitative Analysis:GSAS – General Structural Analysis System is a very mature Rietveld program, and comes in versions to run on Windows/DOS PCs and Linux systems. It has been developed as free open-source software and is maintained and distributed by Allen C. Larson & Robert B. Von Dreele of Los Alamos National Laboratory. It comes with a 231 page manual which contains surprisingly little about Rietveld refinements and is chiefly concerned with how to interact with the 37 different program modules. Written originally for UNIX, the “port” to the Windows platform makes extensive use of Command (i.e., DOS) Windows and behaves much like a bunch of Terminal windows. Initial impressions are quite intimidating, but the software gets great reviews from those who learn to put it through its paces. All versions are available via FTP from ftp://ftp.lanl.gov/public/gsas. We have a recent version available on our FTP site at ftp://eps.unm.edu/pub/xrd/index.htm.FullProf – Another widely used Rietveld system produced by Juan Rodríguez-Carvajal at the Laboratoire Léon Brillouin (CEA-CNRS) in France. Though it has a somewhat friendlier GUI interface than GSAS but is still a complicated analytical tool requiring good data input by a user who understands diffraction data, and crystal structure analysis, and is willing to master fairly complicated input data file structures. The 139-page FullProf 2000 manual (in Acrobat PDF format) includes a good discussion of the Rietveld procedure and suggests the best sequence of steps to follow to produce a good refinement. We have a recent version of FullProf on our ftp site at at ftp://eps.unm.edu/pub/xrd/index.htm. The CCP14 source page for FullProf with tutorial information and links is at http://www.ccp14.ac.uk/tutorial/fullprof/index.html.FULLPAT – Dave Bish and Steve Chiperas Excel-spreadsheet-based whole pattern fitting system uses the Excel solver functions to do a least squares refinement to fit whole- pattern data to standard pattern data to produce quantitative analyses. The program archive consists of two files -- the actual Excel spreadsheet used to do the calculations and a well written 23 page manual that explains the use of the program in sufficient detail to make it usable. It does require rather extensive development of in-house standard XRD patterns prepared using a suitable corundum standard as a "spike". This system was used routinely in Bish and Chiperas well respected LANL XRD lab. Available from CCP14 (http://www.ccp14.ac.uk/ccp/web-mirrors/fullpat/) or on our FTP site at ftp://eps.unm.edu/pub/xrd/index.htm.RockJock – Uses Microsoft Excel Macros and the Solver function to perform a whole-pattern modified Rietveld-type refinement to perform quantitative analysis. Written by Dennis D. Eberl, the software was published in 2003 as U.S.G.S. Open-File Report 03-78, “Determining Quantitative Mineralogy from Powder X-ray Diffration Data”. RockJock requires careful sample preparation, good machine characterization and the use of a ZnO internal standard for best results. It is widely used in clay analyses. Available via FTP from ftp://brrcrftp.cr.usgs.gov/pub/ddeberl/RockJock. (Material in this document is borrowed from many sources; all original material is ©2010 by James R. Connolly)(Revision date: 6-Apr-10) Page 14 of 14